Evaluation of the addition of short coconut fibers on the characteristics of asphalt mixtures
Civil and Environmental Research www.iiste.orgISSN 2224-5790 (Paper) ISSN 2225-0514 (Online)Vol.3, No.4, 201363Evaluation of the addition of short coconut fibers on thecharacteristics of asphalt mixturesSigit Pranowo HadiwardoyoDepartment of Civil Engineering, Universitas Indonesia, UI Campus Depok 16424, Indonesia*E-mail of the corresponding author: email@example.comAbstractThe damage path beginning at the surface layers of the failure receives the load of the traffic and a change intemperature of 20-50 °C. Structural changes in the asphalt mixture cause an increase in the temperature of thesurface of the road, approaching the softening point of asphalt. Short coconut fibers are waste from coconutprocessing, with a length of 5-12.5 mm. The addition of 0.5%, 0.75%, 1%, 1.25%, and 1.50% coconut fiber changedthe characteristics of the asphalt. The fiber size was varied (5, 7.5, 10, and 12.5 mm) to determine its effect on theasphalt characteristics. The fiber size variation was also conducted to determine its effect on the asphalt-aggregatemixture at 60 °C using the Marshall immersion test. The addition of 0.75% 5-mm fibers by weight of the asphaltincreased the value of the Marshall stability by 10-15% and produced a lower penetration-grade bitumen. Thetemperature of the mixing fibers in the asphalt must be below the flash point of the fibers during the heating of theasphalt-fiber mixture.Keywords: coconut fiber, temperature, resilient modulus, asphalt mixtures, Marshall test1. IntroductionIn general, some asphalt mixes for road pavement flow in response to the load due to their plastic deformation athigh temperatures. Such deformation properties accumulate due to repetitive loads. Changes in the surface layers arecause early damage to the road pavement structure.Damage to highways mostly occurs in the top layer, in the binder and erosion layers, rather than the foundation andlower layers. Damage to the binder and erosion layers generally includes surface cracks, deformations, wheel ruts,and potholes (Ozgan, 2011). Damage to roads in Indonesia is caused by environmental factors, overloading, andconstruction. Environmental factors, such as rainfall and road surface temperature changes, are often difficult topredict (Hadiwardoyo et al, 2013). Asphalt obtained from refineries is too soft for paving in high-temperature areasin the summer and too brittle for subzero temperatures in winter in various parts of the country (Attaelmanan et al,2011).As a tropical country, Indonesia has a problem with increases in the road surface temperature. Therefore, a surfacelayer able to resist temperature changes is required. To address this problem, research has been conducted to improvethe performance of asphalt as the road surface layer. One approach is the use of fiber additives mixed into theasphalt. Fiber-added materials are derived from synthetic fiber or natural fiber. Coconut husks are plentiful inIndonesia, which is the producer of 10% of the world demand for coconuts. However, these husks are most readilyavailable as processed waste coconut husks. Standard-sized coconut fibers have been utilized in the coir industry, butshort waste fibers have not yet been utilized. A study conducted by Oda et al (2012) showed that the addition ofcoconut coir fiber increased the resilient modulus by approximately 14%. The coconut is comprised of several parts,including the exocarp, which is a very thin layer covering the fibrous mesocarp. These elements form the bark of thecoconut (approximately 5-mm-thick, depending on the species). Underneath this layer lies the woody endocarp,which is very hard. Natural fibers are cheap and locally available in many countries. Their use as a constructionmaterial to improve the properties of the composites costs very little when compared to the total cost of thecomposites (Ali et al, 2012).The utilization of coconut coir waste can play a role in reducing environmental pollution. Efforts to improve theperformance of asphalt by the addition of natural materials are expected to reduce the ever-increasing need forasphalt as a road construction material. The reduction of the use of natural materials can also be accomplished by
Civil and Environmental Research www.iiste.orgISSN 2224-5790 (Paper) ISSN 2225-0514 (Online)Vol.3, No.4, 201364recycling materials as material additives. The recycling of existing asphalt pavement materials produces newpavements with considerable savings in material use, money, and energy. Aggregate and binder from old asphaltpavement retain their value even after these pavements have reached the end of their service lives (Xiao, 2009).In this study, short coconut fiber is added to asphalt heated to a certain temperature so as to avoid burning thecoconut fiber. The asphalt-fiber characteristics are tested to determine such characteristics as the penetration,softening point, burning point, ductility, density, and Marshall immersion. At high temperatures, the asphalt bindertends to flow more easily due to the natural decrease in viscosity associated with higher temperatures. This conditioncreates a “softer” asphalt mixture, which is prone to rutting (Fontes et al, 2010).The objective of this study was to evaluate the laboratory performance of different sizes of coconut fiber present invirgin asphalt in different percentages. This goal was achieved by evaluating various engineering properties. Thebehavior of coconut fiber asphalt (CFA)-modified mixtures was compared to that of conventional asphalt mixtures.2. Materials and methods2.1. Asphalt cement and aggregateThe aggregate used in the construction of the asphalt sample is derived from Rumpin-Bogor West Java aggregatequarry and grade 60/70 bitumen. The grading of the aggregate can be characterized as influential for the asphaltmixture deformation resistance. Poor aggregate composition refers to the use of too many fine or coarse aggregates,which fails to provide the necessary resistance to deformation.Table 1 Design aggregate gradationSieve Sieve (mm)Passing(%)UndesirablerangeLower-upperlimits¾ in 19 100 - 100½ in 12.5 91 - 90-100⅜ in 9.5 81 - 90No. 4 4.75 59 - -No. 8 2.36 43 39.1 28-58No. 16 1.18 33 25.6-31.6 -No. 30 0.6 25 19.1-23.1 -No. 50 0.3 16 15.5 -No. 200 0.075 6 - 4-10In general, a higher content of fine aggregate and a perfect balance between the distribution of coarse aggregates,fine aggregate, and filler may imbue asphalt mixtures with increased resistance (Mirzahosseini et al, 2011).This study used an asphalt concrete wearing course mix (AC-WC) in which the largest aggregate size was 19 mm.The test results for the characteristics of the coarse aggregate and fine medium are displayed in Tables 1 & 2. Onlyone aggregate gradation shown in Figure 1 was selected for use in the study.The characteristics of asphalt must conform to the requirements specified in the Indonesian standard. Thus, testswere conducted to determine the penetration, ductility at 25 °C, loss due to heat and air, specific gravity, andsoftening point. The physical properties of the asphalt samples are given in Table 3.
Civil and Environmental Research www.iiste.orgISSN 2224-5790 (Paper) ISSN 2225-0514 (Online)Vol.3, No.4, 201365Table 2 Basic properties of the aggregateAggregateMethodValueProperty Coarse Medium FineBulk sp. gr. AASHTO T84/T85 2.52 2.52 2.53Surface saturated dry gravity (SSD) AASHTO T84/T85 2.58 2.59 2.58Apparent sp. gr. AASHTO T84/T85 2.68 2.69 2.66Absorption (%) AASHTO T84/T85 2.40 2.44 2.04Los Angeles abrasion (%) AASHTO T96 18.82 22.12Solubility (%) 98Impact SNI 03-4426-1997 8.54Angularity (%) > 95Toughness (%) BS-812 8.4201020304050607080901000,01 0,10 1,00 10,00percentpassing(%)sieve size (mm)aggregat maximum minimumFigure 1. Aggregate gradationTable 3 Physical properties of asphalt cementProperties of the asphalt cementSpecificationusedPenetration grade 60/70 ASTM D 5Penetration (25 °C, 100 g, 5 s, dmm) 64.39 ASTM D 5Specific gravity 1.087 ASTM D 70Softening point (°C) 48.5 ASTM D 36Flash point (°C) 280 ASTM D 92Ductility (25 °C, 5 cm/min) 110 ASTM D 113
Civil and Environmental Research www.iiste.orgISSN 2224-5790 (Paper) ISSN 2225-0514 (Online)Vol.3, No.4, 2013662.2. Coconut fiber propertiesThe coconut fiber used in this study is derived waste coconut husk for industrial processing. Short coconut fiberswere washed to remove dust and other impurities. The fibers were then dried at 30 °C for 24 h and filtered toseparate the remaining impurities. The physical properties of the short fibers are as follow: length, 5 mm to 12.5 mm;diameter, 0.80-0.15 mm; and density, 600 kg/m3. Short coconut fibers after drying are as shown in Figure 2.Figure 2. Micro-optic coconut fiber images2.3. Coconut fiber-asphalt (CFA) formulationThe coconut coir was cut to lengths of 5 mm, 7.5 mm, 10 mm, and 12.5 mm and added to the bitumen 60/70 in levelsof 0.5%, 0.75%, 1%, 1.25%, and 1.5% by weight of asphalt. The fibers were added upon heating of the asphalttemperature to 150-160 °C by stirring for 5 min until the fibers were evenly mixed. Asphalt fiber can be stored andreheated when used for mixing with aggregate.Fiber size affects the ease of mixing between the asphalt and fiber: the smaller the fiber, the easier the mixingprocess. Coconut fiber will burn before the flash point of asphalt; thus, the mixing of the fibers and asphalt must beperformed below the burning temperature of the coconut fibers.At the end of the test, the fibers were extracted from the bitumen to verify that the coconut fibers did not burn duringthe hot asphalt concrete mixing process. The results show that 96% coconut fiber mixed with bitumen remained aftermixing.2.4. Mix design and optimizationThe content of coconut fiber asphalt in the asphalt concrete mixture is equal to 6.36%. The asphalt was modified andthe aggregate mixed at 155 °C. The samples were then brought to the compaction temperature of 10 °C less than thecorresponding mixing temperature using a Marshall mechanical compactor. The specimens were compacted using 75heavy-duty Marshall blows for each face, corresponding to a tire pressure of 1.379 kPa. Samples with a variety offiber sizes and percentages of the asphalt were tested by Marshall, Marshall immersion, and wheel tracking tests.3. Results and discussion3.1. Rheological testsThe CFA binder rheological properties were evaluated, and the results are presented in Table 4. The results show thatthe CFA is effective in improving the rheological properties of the asphalt cement. Table 4 reveals that the additionof CFA content reduces the penetration and ductility and increases the softening point. The results showed that thesoftening point of CFA modified increased by 2.3% and the penetration decreased by 11.5% with the addition of0.75% coconut fiber (5 mm). The results also reveal that 0.75% CFA decreased the ductility to 47 cm, which showsthat the CFA can still be used in asphalt cement. The increase in the softening point and decrease in the penetrationcan be attributed to the consistency of the CFA binder.
Civil and Environmental Research www.iiste.orgISSN 2224-5790 (Paper) ISSN 2225-0514 (Online)Vol.3, No.4, 2013673.2. Temperature susceptibilityThe penetration index was used to investigate the effect of CFA on the temperature susceptibility of the asphaltmixtures. Figure 3 illustrates the relationship between penetration index and CFA content. All the modified binderswere less susceptible to changes in temperature than virgin asphalt cement. This finding is associated with the highersoftening point and lower penetration value of CFA-modified asphalt compared to virgin asphalt. Figure 3 shows thatthe Penetration Index (P.I.) values for virgin asphalt and 0.75% CFA-modified asphalt are -0.463 and -0.302,respectively. Increased CFA content has increased the P.I., as shown in Figure 3. This important fact shows that CFAmakes the binder less susceptible to temperature and climate.Figure 3. Relationship between size of coconut fiber and penetration index
Civil and Environmental Research www.iiste.orgISSN 2224-5790 (Paper) ISSN 2225-0514 (Online)Vol.3, No.4, 201368Table 4 Basic rheological properties of CFA%coconutfiberLength offiber (mm)Penetration (25 °C,100 g, 5 s, dmm)Ductility (25 °C,5 cm/min)Softeningpoint (°C)Penetrationindex0 - 64.39 110 50.50 -0.4630.50 5.0 53.64 52.33 52.28 -0.4790.50 7.5 57.03 47.50 53.00 -0.1580.50 10.0 56.00 46.47 52.36 -0.3550.50 12.5 57.50 45.90 52.00 -0.3770.75 5.0 57.00 47.57 52.40 -0.3020.75 7.5 61.30 44.33 53.25 0.0860.75 10.0 59.10 44.07 52.95 -0.0800.75 12.5 58.00 43.96 52.85 -0.1511.00 5.0 56.11 44.17 52.42 -0.3361.00 7.5 61.67 42.70 54.46 0.3841.00 10.0 57.00 42.23 53.90 0.0511.00 12.5 58.40 42.10 53.40 -0.0041.25 5.0 59.66 42.17 53.00 -0.0441.25 7.5 61.33 40.50 55.00 0.4931.25 10.0 58.00 40.10 55.00 0.3471.25 12.5 58.60 40.00 54.00 0.1451.50 5.0 60.00 41.70 52.85 -0.0651.50 7.5 62.20 40.10 55.15 0.5651.50 10.0 59.40 39.20 54.90 0.3861.50 12.5 58.75 39.00 53.95 0.1403.3. Influence of coconut fiber on bitumen properties3.3.1. Asphalt penetration valueFigure 4 shows the penetration value of bitumen as a function of coconut fiber length (Figure 4a) and is based on thebitumen content of coconut fiber (Figure 4b). The coconut fiber length affected the penetration value of the asphalt,especially the length of 0.75 cm, which yielded the highest penetration bitumen. Similarly, the percentage content ofcoconut fiber affected the penetration value of the asphalt. A coconut fiber content of 1.5% with a size of 0.75 cmproduced the highest asphalt penetration value, 62.2.
Civil and Environmental Research www.iiste.orgISSN 2224-5790 (Paper) ISSN 2225-0514 (Online)Vol.3, No.4, 201369(a) (b)Figure 4. Relationship between coconut fiber size and asphalt penetration value3.3.2. Softening pointAs shown in Table 4, the softening point of virgin asphalt is 50.5. The addition of coconut fiber in virgin asphaltincreased the softening point by 4-7% for all sizes and contents of coconut fiber in bitumen. Figure 5a shows thatincreases in the percentage coconut fiber in bitumen increased the softening point. Regarding the length of coconutfiber, a length of 0.75 cm yields the best softening point (Figure 5b).(a) (b)Figure 5. Relationship between size of coconut fiber and softening point3.3.3. DuctilityThe addition of coconut fiber has a negative influence on the ductility of the CFA-modified mixtures tested in thisstudy. Table 4 shows that the addition of coconut fiber in the bitumen decreases the ductility, which is 39 for thehighest coconut fiber content studied. The coconut fiber size of 0.5 cm corresponds to the highest CFA ductility
Civil and Environmental Research www.iiste.orgISSN 2224-5790 (Paper) ISSN 2225-0514 (Online)Vol.3, No.4, 201370studied. Figure 6 shows that the longer the coconut fibers and the lower the coconut fiber content, the lower theductility values were.Figure 6. Relationship between CFA content and softening point3.4. Moisture susceptibilityThe adverse effect of moisture on the resistance of asphalt mixtures is expressed by the strength ratio (SR). The SR isdefined as the ratio of dry and wet strength specimens. The higher the SR, the better the resistance to moisturedamage of the asphalt mixtures.Most pavement agencies recommend that the SR value be greater than 70-80% in their mixture design specifications(Roberts et al, 1996).As shown in Table 5, the SR values obtained for both mixtures are greater than 80%, which meets the mixture designspecifications. However, the SR of the CFA-modified (94%) is approximately 2% lower than that of theconventional mixture (96%). An SR value of 94% indicates that negligible moisture damage has occurred in themodified CFA wet specimens. This resistance, which meets the minimum requirements of the modified CFA tomoisture damage, could be mainly attributed to the anti-stripping agent. Figure 7 shows the Marshall stability of dryand wet samples with different contents of coconut fiber.Table 5 Moisture susceptibility resultsCoconutfibercontent(%)Dry WetStrengthratio (%)Airvoid(%)Strength(kPa)Air void(%)Strength(kPa)0 3.49 1,008.7 3.74 970.2 0.960.5 4.14 1,070.3 4.45 1,016.4 0.950.75 3.01 1,332.2 3.43 1,216.7 0.911 3.52 1,209.0 3.99 1,124.2 0.931.25 4.19 1,147.3 4.94 1,062.6 0.931.5 4.57 1,093.4 5.42 1,039.5 0.95The desirable properties of asphalt mixtures for flexible pavement surfacing are stability, durability, flexibility, andskid resistance (Jitsangiam et al, 2013). Conventional hot mix asphalt (HMA) design methods aim to determine theoptimum asphalt content at which the asphalt layer performs satisfactorily, particularly with respect to stability anddurability (Asi et al, 2007).
Civil and Environmental Research www.iiste.orgISSN 2224-5790 (Paper) ISSN 2225-0514 (Online)Vol.3, No.4, 201371Figure 7. Influence of coconut fiber content on Marshall stability3.5. Deformation performance of coconut fiber asphalt mixturesFigure 8 compares the rut depth with the load cycle number for the conventional and CFA-modified mixtures. Theconventional mixture has a maximum rut depth of 1.5 mm after 1260 cycles. In contrast, the maximum rut depth ofthe CFA-modified mixture is approximately 1 mm. It can be concluded that the CFA-modified mixture has thepotential to reduce permanent deformation. Because the aggregate gradation mixture of both mixtures is the same,the increase in resistance to deformation of the CFA-modified mixture is mainly due to the coconut fiber used in themixture.Figure 8. Cumulative rut depths with number of load applications4. ConclusionsThe purpose of this paper was to evaluate the use of short coconut fibers, which are readily available wasteproducts that can disrupt the environment, as an asphalt additive. The results of the use of 5-12.5-mm fibers in theamount of 0-1.5% by weight of asphalt can be summarized as follows:1. The addition of short coconut fiber reduced the penetration grade of bitumen and ductility but increasedthe softening point.
Civil and Environmental Research www.iiste.orgISSN 2224-5790 (Paper) ISSN 2225-0514 (Online)Vol.3, No.4, 2013722. The increase in fiber length caused difficulties in the process of mixing the fibers with asphalt; the shorterthe fiber is, the more the mixing process is facilitated. The 5-mm short coconut fiber yielded the highestductility.3. The test results show that the 0.75% coconut fiber content provided the best performance of the contentsstudied. Additionally, the 0.75% CFA performed better than asphalt mixtures using virgin asphalt.4. CFA extraction test results show that as much as 96% of the fiber is retained, which suggests that coconutfiber does not burn in the asphalt mixing process.AcknowledgmentsThe authors would like to thank everyone who helped them throughout the course of this research, particularly thetechnicians at the Centre of Road Research and Development Laboratory, Ministry of Public Works, Republic ofIndonesia. The assistance of Roberto Colia, Sofiah Indrayani, and Irfan Maulana is very much appreciated.ReferencesAli M, Liu A, Sou H and Chouw Nawawi, (2012): Mechanical and dynamic properties of coconut fibre reinforcedconcrete, Construction Building Materials Vol. 30, p.814-825.Asi IM, (2007): Performance evaluation of SUPERPAVE and Marshall asphalt mix designs to suit Jordan climaticand traffic conditions, Construction Building Materials Vol. 21, p.1732-1740.Ataelmanan M, Feng CP, Al-Hadidy AI. (2011). Laboratory evaluation of HMA with high density polyethylene as amodifier. Journal of Construction Building Materials; 25: 2764-2770.Fonte L.P.T.L., Traches G., Pais J.C., and Pereira P.A.A (2010): Evaluating permanent deformation in asphalt rubbermixtures, Construction Building Materials Vol. 24, p.1993-1200.Hadiwardoyo S.P, Fikri H. (2013): Use of Buton Asphalt Additive on Moisture Damage Sensitivity and RuttingPerformance of Asphalt Mixtures, Civil and Environmental Research Vo. 3 No.3,. P.100-108.Jitsangiam P, Chindaprasirt P and Nikraz. (2013): An evaluation of the stability of SUPERPAVE and Marshallasphalt mix designs as they relate to Thailand’s climatic conditions, Construction Building Materials Vol. 40, p.961-970.Mirzahosseini M.R., Aghaeifar A., Alavi A.H., and Gandomi A.H. (2011): Permanent deformation analysis ofasphalt mixtures using soft computing techniques, Expert Systems with Applications Vol.38, p. 6081-6100.Oda S., Fernandes Jr JL andIldefonso JS (2012): Analysis of use of natural fibers and asphalt rubber binder indiscontinuous asphalt mixtures, Construction Building Materials Vol. 26, p.13-20.Ozgan E, (2011): Artificial neural network based modelling of the Marshall Stability of asphalt concrete. ExpertSystems with Applications Vol.38, p. 6025-6030.Roberts FL, Kandhal PS, Brown ER, Lee D, Kennedy TW. (1996) : Hot mix asphalt materials, mixtures design andconstruction. Lanham (MD) : NAPA Education Foundation.Xiao F, Amirkhanian SN, Shen J and Putman B (2009): Influence of crumb rubber size and type on reclaimedasphalt pavement (RAP) mixtures, Construction Building Materials Vol. 23, p.1028-1034.
Civil and Environmental Research www.iiste.orgISSN 2224-5790 (Paper) ISSN 2225-0514 (Online)Vol.3, No.4, 201373Sigit Pranowo Hadiwardoyo is a doctoral graduate of Ecole Centrale Paris France in 2002, having received hisDiplome Etude Approfondis (DEA) from Ecole Centrale de Lyon France in 1989 and his bachelor degree fromUniversitas Indonesia in 1985. He is also a member of the Indonesian Road Development Association. He is atransportation specialist (highway and railway) with research interests in the performance and improvement ofpavement materials.
This academic article was published by The International Institute for Science,Technology and Education (IISTE). The IISTE is a pioneer in the Open AccessPublishing service based in the U.S. and Europe. The aim of the institute isAccelerating Global Knowledge Sharing.More information about the publisher can be found in the IISTE’s homepage:http://www.iiste.orgCALL FOR PAPERSThe IISTE is currently hosting more than 30 peer-reviewed academic journals andcollaborating with academic institutions around the world. There’s no deadline forsubmission. Prospective authors of IISTE journals can find the submissioninstruction on the following page: http://www.iiste.org/Journals/The IISTE editorial team promises to the review and publish all the qualifiedsubmissions in a fast manner. All the journals articles are available online to thereaders all over the world without financial, legal, or technical barriers other thanthose inseparable from gaining access to the internet itself. Printed version of thejournals is also available upon request of readers and authors.IISTE Knowledge Sharing PartnersEBSCO, Index Copernicus, Ulrichs Periodicals Directory, JournalTOCS, PKP OpenArchives Harvester, Bielefeld Academic Search Engine, ElektronischeZeitschriftenbibliothek EZB, Open J-Gate, OCLC WorldCat, Universe DigtialLibrary , NewJour, Google Scholar